# diffusion in solids ... solids ¢â‚¬â€œ vacancy diffusion or...

Post on 25-Sep-2020

0 views

Embed Size (px)

TRANSCRIPT

17 March 2015

Diffusion in Solids

ELEC3215 Fluids and Mechanical Materials

Pt 3 Electromechanical Engineering

• C

changes as we solidify. • Cu-Ni case:

• Fast rate of cooling: Cored structure

• Slow rate of cooling: Equilibrium structure

First

to solidify has C

= 46 wt% Ni. Last

to solidify has C

= 35 wt% Ni.

Cored vs Equilibrium Phases

First to solidify: 46 wt% Ni

Uniform C: 35 wt% Ni

Last to solidify: < 35 wt% Ni

Diffusion and Kinetics of Phase Transformation are important!

ISSUES TO ADDRESS...

• How does diffusion occur?

• Why is it an important part of processing?

• How can the rate of diffusion be predicted for some simple cases?

• How does diffusion depend on structure and temperature?

Diffusion in Solids

Diffusion

Diffusion - Mass transport by atomic motion

Mechanisms

Gases & Liquids – random (Brownian) motion

Solids – vacancy diffusion or interstitial diffusion

• Interdiffusion: In an alloy, atoms tend to migrate from regions of high concentration to regions of low concentration

Initially

Diffusion

After some time

• Self-diffusion: In an elemental solid, atoms also migrate.

Label some atoms After some time

Diffusion

A

B

C

D A

B

C

D

Mechanisms:

Diffusion Mechanisms

Vacancy Diffusion: • atoms exchange with vacancies • applies to substitutional impurities atoms • rate depends on:

--number of vacancies --activation energy to exchange.

increasing elapsed time

Diffusion Mechanisms

Interstitial diffusion – smaller atoms can diffuse between atoms.

More rapid than vacancy diffusion

• Case Hardening: --Diffuse carbon atoms

into the host iron atoms at the surface.

--Example of interstitial diffusion is a case hardened gear.

• Result: The presence of C atoms makes iron (steel) harder.

Processing Using Diffusion

• Doping silicon with phosphorus for n-type semiconductors: • Process:

3. Result: Doped semiconductor regions.

silicon

Processing Using Diffusion

magnified image of a computer chip

0.5mm

light regions: Si atoms

light regions: Al atoms

2. Heat it.

1. Deposit P rich layers on surface.

silicon

Doped region need to be interconnected !

• What material to choose? Cu, Ag, Au, Al ? • Process involves further heat treatments.

Conducting circuit paths

Al is the best choice in spite of lower electric conductivity

Cu can be use but thin barrier layer of Ta has to be deposited first ( cost ! )

Diffusion

How do we quantify the amount or rate of diffusion?

Measured empirically

Make thin film (membrane) of known surface area

Impose concentration gradient

Measure how fast atoms or molecules diffuse through the membrane

sm kgor

scm mol

timearea surface diffusing mass) (or molesFlux 22J

1M dMJ At A dt

M = mass

diffused time

J

slope

Geometry of Fick’s first law

Steady-State Diffusion

dx dCDJ

Fick’s first law of diffusionC1

C2

x

C1

C2

x1 x2

D

diffusion coefficient

Rate of diffusion independent of time Flux proportional to concentration gradient =

dx dC

12

12 linear if xx CC

x C

dx dC

Example: Chemical Protective Clothing (CPC)

Methylene chloride is a common ingredient of paint removers. Besides being an irritant, it also may be absorbed through skin. When using this paint remover, protective gloves should be worn.

If butyl rubber gloves (0.04 cm thick) are used, what is the diffusive flux of methylene chloride through the glove?

Data: diffusion coefficient in butyl rubber:

D = 110x10-8 cm2/s surface concentrations:

C2 = 0.02 g/cm3 C1 = 0.44 g/cm3

scm g 10 x 16.1

cm) 04.0( )g/cm 44.0g/cm 02.0(/s)cm 10 x 110( 2

5- 33

28-

J

Example (cont).

12

12- xx CCD

dx dCDJ

D

tb 6

2

glove C1

C2

skinpaint remover

x1 x2

• Solution – assuming linear conc. gradient

D = 110x10-8 cm2/s

C2 = 0.02 g/cm3 C1 = 0.44 g/cm3

x2 – x1 = 0.04 cm

Data:

Thermal Activation

Process path showing how an atom must overcome an activation energy, q, to move from one stable position to a similar adjacent position

/( )"jump" rate * Bq k Tconst e

Diffusion and Temperature

• Diffusion coefficient increases with increasing T.

D Do exp

Qd RT

= pre-exponential [m2/s] = diffusion coefficient [m2/s]

= activation energy [J/mol or eV/atom] = gas constant [8.314 J/mol-K] = absolute temperature [K]

D Do Qd R T

Diffusion and Temperature

D has exponential dependence on T

Dinterstitial >> Dsubstitutional C in -Fe C in -Fe

Al in Al Fe in -Fe Fe in -Fe

1000K/T

D (m2/s) C in -Fe

C in -Fe

Al in Al

Fe in -Fe

Fe in -Fe

0.5 1.0 1.5 10-20

10-14

10-8 T(C)15

00

10 00

60 0

30 0

Alternative Diffusion Paths

Self-diffusion coefficients for silver depend on the diffusion path

In general, diffusivity is greater through less- restrictive structural regions Surfaces Grain boundaries

(Lattice)

Diffusion at Micro scale

Schematic illustration of how a coating of impurity B can penetrate more deeply into grain boundaries and even further along a free surface of polycrystalline A, consistent with the relative values of diffusion coefficients

(Dvolume < Dgrain boundary < Dsurface )

Effect of Grain Boundaries

Represent a grain by a cylinder: diameter d with grain boundary width .

Area of grain =

Area of grain boundary =

Hence ratio of areas is

2 lattice gbD D D d

“Top view”

22d 2

2 2 d 2

d

lattice lattice gb gbJ A J A J A

2 lattice gbJ J J d

Effect of Grain Boundaries

Grain boundaries have a more open structure, so Qgb < Qlattice

Should result in faster diffusion in polycrystalline samples than in single crystals.

However, the grain boundary area forms such a small fraction of the total area

The effect is only significant at low temperatures, when Dlattice

Example: At 300ºC the diffusion coefficient and activation energy for Cu in Si are

D(300ºC) = 7.8 x 10-11 m2/s Qd = 41.5 kJ/mol

What is the diffusion coefficient at 350ºC?

1 01

2 02

1lnln and 1lnln TR

QDD TR

QDD dd

121

2 12

11lnlnln TTR

Q D DDD d

transform data

D

Temp = T

ln D

1/T

Example (cont.)

K 573 1

K 623 1

K-J/mol 314.8 J/mol 500,41exp /s)m 10 x 8.7( 2112D

12 12

11exp TTR

QDD d

T1 = 273 + 300 = 573K T2 = 273 + 350 = 623K

D2 = 15.7 x 10-11 m2/s

Non-steady State Diffusion

The concentration of diffucing species is a function of both time and position C = C(x,t)

In this case Fick’s Second Law is used

2

2

x CD

t C

Fick’s Second Law

Profile changes in time!Steady State: Fixed profile

v.s.

Non-steady State Diffusion

B.C. at t = 0, C = Co for 0

x

at t > 0, C = CS for x = 0 (const. surf. conc.)

C = Co for x =

• Copper diffuses into a bar of aluminum.

pre-exi